(2) International Research Journal of Engineering and Technology (IRJET). e-ISSN: 2395-0056. Volume: 06 Issue: 05 | May 2019. p-ISSN: 2395-0072. www.irjet.net. 1.2 Preparation of Aluminium alloy Composites The stir casting method was used develop the reinforcement metal matrix composites with the temperature of stir casting furnace was maintained at 7000C. AL 7075 is first put into the crucible and furnace is closed. After twenty minutes, the metals were verified for their molten state and after the confirmation, the metals such as boron carbide and graphite were put inside and the furnace was closed. After 15 to 20 minutes, the boron carbide and graphite was added and the aluminium stirrer was set to 550 rpm and it rotates. After the stirrer is rotated for about five minutes, the stirrer was stopped and the molten metal was taken out. It was kept in cooling nature for about two hours. Base Material. B4C (%). Gr (%). Stir Speed (rpm). Stir Time (mins). Pouring Temp. (C). Preheated Temp. (C). Al-7075. 4. 4. 550. 5. 700. 350. 2. Testing of Composites Microstructure study has been carried out on the prepared composite using Vegas Tescan made scanning electron microscope. Basically the test samples of 10-12mm in diameter are cut from the prepared castings using lathe machine and are polished thoroughly as already mention methods it is etched using reagent for better results. The polished specimens which looks like mirror. The specimens are characterized for various magnifications (100X, 200X, 800X) to indicate distribution of reinforcements in metal matrix. The microstructures of samples i.e. as cast, 4 wt% B 4C and 4wt% of Graphite are also examined. Tensile test specimens were machined from the cast samples. The tensile specimens of circular cross section with a diameter of 9 mm and gauge length of 45mm were prepared according to the ASTM E8 standard testing procedure using Instron made Universal Testing Machine. All the tests were conducted in a displacement control mode at a rate of 0.1 mm/min. Multiple tests were conducted and the best results were averaged. Various tensile properties like ultimate tensile strength, yield strength and percentage elongation were evaluated for as cast Aluminium alloy. Figure 1 showing the tensile test specimen dimensions used to conduct the experiments.. Figure 1: Tensile specimen and its dimensions in mm Results and Discussion Microstructure Study. (a) © 2019, IRJET. |. Impact Factor value: 7.211. (b) |. ISO 9001:2008 Certified Journal. |. Page 5205.
(3) International Research Journal of Engineering and Technology (IRJET). e-ISSN: 2395-0056. Volume: 06 Issue: 05 | May 2019. p-ISSN: 2395-0072. www.irjet.net. (c). (d). Figure 2: Showing the Scanning Electron Microscope image of Al-7075alloy(a) and 4%B4C+4%Gr (b) Figure 2 (a) shows the SEM microphotographs of Aluminium alloy as cast. Fig. 2 (b) clearly shows and even distribution of B4C in the Aluminium alloy matrix. similarly ,Fig 2 (c) clearly shows and even distribution of Gr and Fig 2 (d) clearly shows and even distribution of Aluminium with 4 wt. % B4C+4%Gr particulate. There is no evidence of casting defects such as porosity, shrinkages, slag inclusion and cracks which is indicative of sound castings. In this, wetting effect between particles and molten Aluminium alloy matrix also retards the movement of the reinforcement thus, the particles can remain suspended for a long time in the melt leading to uniform distribution.. Figure 3: Eneregy Dispersive Spectrograph of Aluminium Alloy. Figure 3: Eneregy Dispersive Spectrograph of Hybrid Aluminium Alloy © 2019, IRJET. |. Impact Factor value: 7.211. |. ISO 9001:2008 Certified Journal. |. Page 5206.
(4) International Research Journal of Engineering and Technology (IRJET). e-ISSN: 2395-0056. Volume: 06 Issue: 05 | May 2019. p-ISSN: 2395-0072. www.irjet.net. In order to confirm the presence of B4C+4%Gr energy dispersive spectroscope analysis was carried out at the edge of the reinforcement particle and Aluminium alloy matrix. The EDS spectrum reveals the presence of Al, Zn, Cu and Mg in the interface reaction layer. Tensile Properties After the test is completed the results are taken on an average and mentioned. We see that the values are increasing as we add the reinforcements to the aluminium alloy. We achieve a maximum tensile stress of 248.88 MPa for Hybrid composite material. We can easily make out the difference that upon addition of reinforcements there is gradual increase in trend for yield strength. This is because reinforcements act as obstacles to the moment of dislocations and also upon adding the Graphite into molten metal it increases the elongation properties there by yielding more which in turn yield strength increased.. Stress in MPa. Ultimate Tensile Strength 260 250 240 230 220 210 200 190. 226.36. Al7075-4% B4C. Al7075-4% Graphite. 212.45 Al7075. 248.88. 226.49. Al7075-4% B4C+4% Graphite. Figure 4a: Ultimate tensile strength of Hybrid Aluminium alloy composites. Stress in MPa. Yield Strength 210 200 190 180 170 160 150. 189.38. 185.26. Al7075-4% B4C. Al7075-4% Graphite. 172.34 Al7075. 198.46. Al7075-4% B4C+4% Graphite. Figure 4b: Yield strength of Hybrid Aluminium alloy composites. Hardness Study The Brinell hardness test on all compositions was conducted using steel ball indenter at an applied load of 60kgf for time of 10 seconds to each sample at different locations. We can see that the hardness values are greater than that of its aluminium alloy. It is clear that hardness values are decreasing due to graphite contenting the alloy. Drop of hardness values due to softness of the graphite, which is soft do not contribute for hardness of the composite as they won’t act as barriers for the dislocations moment within the matrix but Boron Carbides does contrary; since B 4C particles which are ceramics having much higher hardness than the base matrix, they obstruct dislocations. The observations made are consistent Increased in the hardness of composites reinforced with B4C and Gr has been reported by several workers. © 2019, IRJET. |. Impact Factor value: 7.211. |. ISO 9001:2008 Certified Journal. |. Page 5207.
(5) e-ISSN: 2395-0056. Volume: 06 Issue: 05 | May 2019. p-ISSN: 2395-0072. Brinell Hardness Number. International Research Journal of Engineering and Technology (IRJET) www.irjet.net. Hardness 85 80 75 70 65 60 55. 79.6. 78.2. 69.6 Al7075. Al7075-4% B4C. 66.5 Al7075-4% Graphite. Figure 5: Hardness of Hybrid Aluminium alloy composites. Al7075-4% B Graphit. 3. CONCLUSIONS The mechanical investigations of the Aluminium alloy composites materials produced by stir casting are remarked as below: . The liquid metallurgy technique was successfully adopted in the preparation of Aluminium alloy composites. The microstructural studies revealed the uniform distribution of the B4C and Gr particulates in the Aluminium alloy matrix. The ultimate tensile strength and yield strength properties of the composites found to be higher than that of base matrix. Improvements in hardness of the Aluminium alloy matrix were obtained with the addition of B4C and Gr particulates.. REFERENCES . Kenneth Kanayo Alaneme and Kazeem Oladiti Sanusi, Engineering Science and Technology, an International Journal, 18(3), 416(2015). . S. Nallusamy and A. Karthikeyan, Indian Journal of Science and Technology, 9(35), 01(2016). . A. Karthikeyan and S. Nallusamy, Int. Journal of Engineering Research in Africa, 31, 36(2017). . Viney Kumara, Rahul Dev Guptab and N.K. Batrab, Procedia Materials Science, 6, 1365(2014). . S. Nallusamy and Gautam Majumdar, Int. Journal of Performability Engg., 12(3), 229(2016). . R. Suganthini Rekha, S. Nallusamy, R. Vijayakumar and S. Saravanan, International Journal of Applied Engineering Research, 10(62), 133(2015). . G. Ramanan, Dhas, Ramachandran and Samuel, Rasayan Journal of Chemistry, 10(2), 375(2017). . S. Nallusamy and A. Karthikeyan, Journal of Nano Research, 49, 01(2017). . Rajesh Prabha, N and Edwin Raja Dhas, J, Rasayan Journal of Chemistry, 10(3), 729(2017). . S. Nallusamy and Saurabh Kumar, Indian Journal of Science and Technology, 9(16), 01(2016) 11. S. Jeevanantham, N.M. Sivaram, D.S. Robinson Smart, S. Nallusamy and N. Manikanda Prabu.. © 2019, IRJET. |. Impact Factor value: 7.211. |. ISO 9001:2008 Certified Journal. |. Page 5208.